pinch-off. This behaviour can be explained by that the depletion region formed at
the drain contact grows and eventually becomes comparable to the channel
length as the drain voltage is increased. This leads to a reduction and drain
voltage dependence of the effective channel length (L’). Thus, since the drain
current is inversely proportional to the channel length, the drain current will
increase with the drain voltage when the transistor is operated beyond pinch-off.
This short-channel effect is called channel-length modulation (CLM). This effect
can be accounted for, to a first approximation, by adding the term (1 + λV
the equation for the drain current in the saturation regime. The constant λ is
called the channel-length modulation parameter.
Some other short-channel effects can be observed in the transfer
characteristics. A reduction in the channel length can lead to an increased and
drain voltage dependent subthreshold current, which reduces the on/off current
ratio. A drain voltage dependent shift in the threshold voltage can also be
observed. This short-channel effect is called threshold voltage roll-off and is
common in inorganic field-effect transistors.
If the longitudinal electric field becomes very high, the drain current may
become dominated by a space-charge limited current (SCLC) flowing through
the bulk of the semiconductor.
This will give the transistor diode-like output
characteristics that can be described by
, where n ≥ 2.
Short-channel effects can be avoided by keeping the transverse electric field
much larger than the longitudinal electric field. That is normally accomplished
by reducing the thickness of the gate insulator with a least the same factor as the
channel length is reduced.
4.7 Gate Insulator Materials
Charge transport in the transistor channel takes place at, or very close to, the gate
insulator-semiconductor interface. Thus, the properties of the interface and the
gate insulator can have a huge influence on the transistor characteristics.
been reported that high-permittivity gate insulators can induce additional
energetic disorder in the channel that enhances carrier localization and leads to a
reduction of the charge carrier mobility.
Thus, using a low-permittivity gate
insulator material can improve the performance of a transistor. It has also been
shown that hydroxyl groups at the insulator interface, e.g. in SiO
, create electron
traps that inhibit n-channel conduction.
However, with hydroxyl-free gate
insulators, such as polyethylene (PE) or benzocyclobutene derivatives (BCB), n-
channel behaviour can in fact be observed in most organic semiconductors.
4.7.1 Low-Voltage Operation
Many of the envisioned applications for organic electronics will require
transistors that are capable of operating at a low supply voltage. Low-voltage
operation is accomplished by employing a gate insulator layer that has a high
capacitance. Traditionally, this is done by reducing the thickness (d) of the gate
, by employing a gate insulator material with high permittivity
or by a combination of the two approaches (see Eq. 4.1). Organic
materials typically have low permittivity,
so it has also been common to use
inorganic high-κ materials, e.g. oxides, as the gate insulator.
One of the most
studied high-capacitance systems, used for TFTs with bottom-gate architecture,
is the combination of a thin oxide (e.g. SiO
) and a self-assembled
monolayer (SAM), which can provide a capacitance up to 1 µF cm
Such transistors can be operated with voltages of just a few volts.
Alternatively, instead of an electrically insulating dielectric material, an
ionically conducting electrolyte can be used as the gate insulator material. This
concept is far from new. The first organic transistor, demonstrated already in
1984, used a liquid electrolyte.
A few years later, in 1987, the same research
group also made the first organic thin-film transistors including a solid-state
electrolyte gate insulator.
Since then, n- and p-channel electrolyte-gated
organic transistors based on a large variation of electrolyte systems, including
have been reported. These transistors can be
classified as being either field-effect transistors or electrochemical transistors,
which will be further discussed in section 4.7.3.
4.7.2 Electrolytic Gate Insulators
A dielectric and an electrolytic gate insulator are compared in Figure 4.6. The
figure schematically illustrates the voltage profile and the electric field
distribution inside the two gate insulator materials when a negative voltage (V) is
applied to the gate electrode.
Figure 4.6 Schematic cross section of an organic thin-film transistor and
illustrations of the voltage (V) and electric field (E) distributions in a dielectric and
an electrolytic gate insulator when a negative gate voltage is applied.
In the case of a dielectric gate insulator, the electrostatic potential will drop
linearly across the insulator layer and, consequently, it produces a constant,
uniform electric field (E = –V/d) throughout the layer.
The static charge polarization mechanism in the electrolytic gate capacitor is
essentially identical to that described for the electrolytic capacitors including two
metal electrodes (see chapter 3). The only difference now is that a semiconductor
represents one of the electrodes. Thus, the ions will redistribute to form EDLs at
the gate-electrolyte and at the electrolyte-semiconductor interfaces, with a
charge-neutral electrolyte in between them. Practically all the applied voltage
will be dropped across the EDLs. The electric field will therefore be very high at
the interfaces, on the order of 10
, and negligible inside the electrolyte
bulk. A high transversal electric field has been shown to suppress short-channel
effects in polyelectrolyte-gated transistors with submicrometer channel
The total capacitance of the electrolyte layer is determined by the capacitance
of the two EDLs connected in series. Thus, the total capacitance will never be
larger than the smaller of the two EDL capacitors, which usually is the EDL at
the electrolyte-semiconductor interface. The capacitance is typically on the order
of 10 µF cm
, which thus makes it possible to induce a very large charge carrier
) in the transistor channel at a relatively low applied
gate voltages (< 3 V).
Moreover, the static capacitance of the electrolyte is
virtually independent on the thickness of the layer,
which means that
relatively thick electrolyte layers can be used to attain low-voltage operation.
This is a huge advantage when it comes to manufacturing, e.g. using roll-to-roll
production. In particular, this makes this class of transistors attractive for printed
electronics applications. However, the transistor will become slower as the
thickness is increased.
V E V E
4.7.3 Operating Modes in Electrolyte-Gated Transistors
It has been debated whether operating mechanism in electrolyte-gated transistors
is electrostatic charging (field-effect) or electrochemical doping. In these
transistors, the induced charges in the channel are balanced by ions in the
electrolyte layer. In this sense, the organic semiconductor can be considered to be
electrochemically doped. On the other hand, in an ideal EDL, the ionic and
electronic charges are separated at the interface and compose oppositely charged
sheets, in between which a uniform electric field is formed. So in this sense, the
semiconductor can be considered being electrostatically charged. Thus, an
electrolyte-gated transistor that forms ideal EDLs (Fig. 4.7a) can be viewed as
both an electrochemical and a field-effect transistor, since it resides at the border
between the two kinds. However, electrolyte-gated transistors, in which the ions
are transferred across the EDL and cause electrochemical doping of the
semiconductor bulk (Fig. 4.7b), are evidently not field-effect transistors. Hence,
in order to distinguish between these to types of electrolyte-gated transistors, the
first is referred to as an organic field-effect transistor (OFET) and the second as
an organic electrochemical transistor (OECT). This notation is kept throughout
the papers that are included in this thesis.
In the OECT, doping of the semiconductor produces a significant increase of
the drain current since the channel becomes three-dimensional, which can be
advantageous in some applications.
However, turning an OECT on and off
will involve transport of ions in and out of the semiconductor bulk, which
typically gives the OECT a more sluggish switching behaviour as compared to an
Some electrolyte-gated transistors are designed to work in the
while other transistors become unintentionally doped
under certain circumstances. For example, a gradual transition from a field-effect
mode to an electrochemical mode, as the gate voltage is increased, has been
observed in transistors gated with polymer electrolytes
and also in
transistors gated via ion gels.
However, employing a polyelectrolyte gate
insulator can suppress parasitic bulk doping of the organic semiconductor and
ensure field-effect operation.
Figure 4.7 Schematic illustration of an electrolyte-gated organic thin-film
transistor operating in (a) the field-effect and (b) in the electrochemical mode.
4.8 Integrated Circuits
One of the main application areas for transistors is as the signal-processing
element in electronic circuits. In many senses, the most basic integrated circuit is
the voltage inverter, which inverts an incoming signal V
into an outgoing signal
. The inverter is also a basic building block in digital electronics, where it is
commonly referred to as a NOT gate. The analysis of an inverter can be used for
predicting the behaviour of more complex gates such as NAND and NOR gates,
which in turn are basic building blocks for more advanced circuits, such as
4.8.1 Inverter Parameters
The transfer characteristics (V
) for an inverter are displayed in
Figure 4.8. From this graph, it is possible to extract the device parameters such as
voltage amplification, or gain, noise margins and operating logic levels. The gain
is defined as
The inverter needs to have a voltage gain larger than unity in order to drive other
subsequent gates. The switching threshold voltage V
is the point in the transfer
curve where the output and input voltages are equal. Ideally, this value is equal to
half the applied supply voltage (V
). The parameters V
are the high
and low values of the output voltage, respectively. The voltage swing (V
) of the gate should be as large as possible, ideally V
. The parameters V
are defined as the operating point were g = –1. The noise margins for low
and high inputs are given by NM
respectively. The noise margins are measures of the robustness of the inverter
and should consequently be as large as possible. A high gain will normally
generate large noise margins.
An inverter can be constructed with only transistors using either a unipolar or a
complementary circuit design.
4.8.2 Unipolar Circuits
Unipolar circuits are composed of transistors of one and the same type, that is,
the circuit only includes either p-channel or n-channel transistors. The circuit
diagram for the two most common unipolar inverter designs are shown in Figure
4.9a and b. Both inverters include two enhancement-mode transistors that are
connected in series. One of them represents the driver transistor and the other is
the load transistor. In both designs, the input and output nodes are connected to
the gate and drain contacts of the driver transistor, respectively. The gate
Figure 4.8 Transfer characteristics for an inverter with annotations of the most
common inverter parameters.
Figure 4.9 Circuit schematics of inverters with unipolar (p-channel) and
complementary designs: (a) unipolar inverter with saturated load; (b) unipolar
inverter with depleted load; (c) complementary inverter based one p-channel (top)
and one n-channel (bottom) transistor.
electrode of the load transistor is either connected to its drain or to its source
electrode. In the former case, the load transistor is operated in the saturation
regime and the device is therefore called a saturated load inverter (Fig. 4.9a). In
the latter case, the load transistor is always switched off. Thus, the device can be
denoted to as a depleted load inverter (Fig. 4.9b). The load transistor in this
design should preferably be a depletion-mode transistor.
Due to a more constant resistance of the load transistor, the depleted load
inverter typically gives better static characteristics as compared to the saturated
However, one downside with both these inverters is the high
power dissipation due to the low resistance of the circuit at high input voltage.
input voltage, V
output voltage, VOUT
g = –1
g = –1
(a) (b) (c)
4.8.3 Complementary Circuits
Complementary circuits includes both n- and p-channel transistors (n- and p-
TFTs), both of enhancement-mode type. That means that the threshold voltages
of the n-TFTs and the p-TFTs are positive and negative, respectively. That is,
< 0 and V
> 0. Complementary circuits are usually designed so that
only positive voltages are used.
The circuit diagram of a complementary inverter is given in Figure 4.9c. The
gate electrodes of the two TFTs are connected and serve as the input node to the
inverter. The drain electrodes of the two transistors are also connected and serve
as the output node. The source electrode of the n-TFT is connected to ground and
the source electrode of the p-TFT is connected to the power supply (V
effective gate-source and drain-source voltages for the p-TFT are thus V
For a low input (e.g. V
= 0), the n-TFT will be OFF (V
= 0 < V
) and the
p-TFT will be ON (|V
| = V
|). The output node will then be charged to
through the p-TFT.
For a high input (e.g. V
), the n-TFT will be ON (V
and the p-TFT will be OFF (|V
| = 0 < |V
|). The output node will then be
discharged to ground through the n-TFT.
Note that only one of the TFTs is on in each of these two logic states. The
current flow from the power supply to ground, through the transistors, will
therefore be low, and limited by the off-current of the transistor that is in the off-
state. A considerable current will only be conducted during the short transition
period between the two logic states, when both transistors are slightly on. Thus,
the static power dissipation is very low.
Other benefits are full rail-to-rail
voltage swing, low output impedance, high gain and high noise margins. Hence,
complementary circuits are essentially better than unipolar circuits in every
aspect, and that is simply why this technology is so dominating today.
4.8.4 Ring Oscillators
A practical method for evaluating the dynamic performance of an integrated
circuit technology, and also the included transistors, is to fabricate so-called ring
oscillator circuits. A ring oscillator consists of an odd number of inverters that
are connected in series, in a loop (Fig. 4.10). Due to the odd number of gates, the
circuit will begin to oscillate between two voltage levels when a supply voltage
is applied. In the loop, at least one of the inverters is switching its logic output
state at a given time. Then, the subsequent gate will switch, and so on. The
oscillation can be monitored by measuring the voltage at an output node of one
of the inverters. An extra inverter can also be connected to this output node in
order to prevent that the actual measurement influences the oscillation. The
period of the oscillation corresponds to the time it takes for a logic state to be
changed twice of each inverter. Thus, the signal propagation delay per stage is
where n is the number inverters and f the frequency of the oscillation. As was
pointed out in section 4.4, the signal delay is normally inversely proportional to
the cutoff frequency.
Figure 4.10 Schematic illustration of a five-stage ring oscillator with output buffer.
5 Manufacturing and Characterization of
The electrolyte-gated transistors that are reported in the papers included in this
thesis are manufactured using different materials and methods. The ambition of
this chapter is not to describe all of them, but to give a general description of
how an electrolyte-gated transistor is manufactured, and also how it can be
5.1 Device Fabrication
The transistor devices were fabricated in a cleanroom (class 1000-10000). All
process steps were carried out in ambient atmosphere and at room temperature
unless otherwise noted. All the transistors reported in the included papers have a
top-gate bottom-contact configuration, but only the transistors in Paper I–IV are
true thin-film transistors, since they include semiconductors, gate insulators and
electrodes as thin layers on planar substrates. The general manufacturing route of
such polyelectrolyte-gated organic thin-film transistors is presented below.
For simplicity, the thin-film transistors are fabricated on rigid and planar
surfaces. Borosilicate glass (Corning 7059 or DESAG D263) and silicon wafers
with a thermally grown silicon dioxide (SiO
) layer are therefore used as the
substrates. However, it should be possible to use a flexible substrate, such as a
plastic foil, as well. The substrates are carefully cleaned with solvents and then
dried before further processing is performed.
5.1.2 Source and Drain Electrodes
The source and drain electrodes are patterned by traditional photolithography and
wet chemical etching processing, as illustrated in Figure 5.1. First, global layers
of ~5 nm chromium (as adhesion layer) and 30–60 nm gold are vacuum
deposited (thermal evaporation). A uniform positive photoresist layer (0.5 µm)
Figure 5.1 Schematic illustration of photolithographic patterning of a metal layer.
is then spin-coated on top of the metal layer and is thereafter soft-baked on a hot
plate, under vacuum, in order to remove residual solvent. The photoresist layer is
then exposed with UV-light through a photomask, which has the desired
electrode pattern. The exposed areas of the photoresist are dissolved in a
developer. The remaining photoresist will thus have the same pattern as the
mask. The uncovered gold is removed by wet etching in an aqueous solution
based on potassium iodide and iodine. The remaining photoresist is then
removed. As a last step, the exposed parts of the thin chromium layer are
removed by wet etching in a solution containing ceric ammonium nitrate, using
the patterned gold electrodes as a mask.
The source and drain electrodes of the transistors in Paper I and II are
relatively large (~500 µm wide) and have simple rectangular geometries that
together form a single rectangular channel. The source and drain electrodes in the
transistors in Paper III and IV, on the other hand, are very narrow (~3.5 µm
wide) and form multiple parallel channels.
5.1.3 Organic Semiconductor Layer
The organic semiconductors (soluble conjugated polymer are here used) are
dissolved in chlorinated solvents, such as chloroform or ortho-dichlorobenzene,
at a concentration of 3–10 mg ml
. The solution is heated and then filtered with
a hydrophobic polytetrafluoroethylene (PTFE) syringe filter with a pore size of
0.1–0.2 µm. The organic semiconductor layer is formed by spin-coating, which
typically gives a film thickness ranging from 10 to 40 nm. The film is then dried
at 60 to 80 °C under dry nitrogen atmosphere, resulting in a semicrystalline film.
5.1.4 Electrolytic Gate Insulator Layer
The polyelectroytes are typically received as highly concentrated (≥ 30 wt%)
water solutions. The solutions are first diluted with n-propanol and deionized
water to give a concentration of ~10–40 mg ml
. Thus, the solvent is then a
mixture of n-propanol and water, containing mostly n-propanol (75–80 %). The
high concentration of the alcohol part is needed in order to make the solution wet
the strongly hydrophobic semiconductor surface. Finally, the solution is filtered
before it is processed using a syringe filter having a pore size of 0.1 µm. The
polyelectrolyte solution is then spin-coated in nitrogen, giving a film thickness of
50–100 nm. The polyelectrolyte layers are then annealed on a hot plate under
vacuum at 110 °C for 90 s.
5.1.5 Gate Electrode
Titanium gate electrodes (80–100 nm thick) are formed by thermal evaporation
through a shadow mask. A simple polyimide (Kapton®) mask is used for the
transistors that have simple rectangular source-drain electrodes (Paper I and II).
The mask is aligned and attached to the sample manually. An electroplated nickel
mask is used for the transistors that have interdigitated source-drain electrodes
(Paper III and IV). The alignment of this opaque mask requires a transparent
substrate, e.g. glass, because the sample is positioned upside-down, on top of the
mask and is simply aligned by manoeuvring the sample in to place, by hand. The
alignment is done with the help of a microscope, which allows for alignment
accuracy better than 20 µm. Microscopy images of the two different kinds of
transistors are shown in Figure 5.2.
5.1.6 Integrated Circuits
In unipolar circuits, p- or n-channel transistors are manufactured side by side. In
order to make integrated circuits, all uncovered organic material around the
transistors is removed by reactive-ion etching (O
, Ar), using the titanium
gate electrodes as hard masks. Interconnects between the source, drain and gate
electrodes are then formed by thermal evaporation through another shadow mask,
which complete the circuits. A microscopy image of a unipolar integrated circuit
is shown in Figure 5.3a.
Complementary circuits are made using the same manufacturing procedure as
described above. The p-channel transistors are manufactured first and then dry
etched to remove the exposed organic materials. Further, a fluorinated polymer is
patterned on top of this first set of transistors in order to protect them from the
solvents used in the subsequent process steps. The n-channel transistors are then
manufactured next to the first set of transistors. All exposed organic materials,
including the fluorinated protective layer, are then removed using reactive-ion
etching. Thereafter, interconnects are formed by vacuum deposition through a
shadow mask. A microscopy image of a complementary integrated circuit is
shown in Figure 5.3b.
Figure 5.2 Microscope images of polyelectrolyte-gated thin-film transistors. (a)
Single-channel transistor having a large parasitic electrode overlap. (b) Dual-
channel transistor with interdigitated source and drain electrodes having a small
parasitic electrode overlap.
Figure 5.3 Microscope images of two integrated circuits based on
polyelectrolyte-gated thin-film transistors. Seven-stage ring oscillator with output
buffer with (a) unipolar design and (b) complementary design.
5.2 Electrical Characterization
In all the electrical measurements, the sample to be tested is placed on a
grounded plate. Micromanipulators are used for contacting the metal electrodes
on the sample, and coaxial or triaxial cables are used between the electrical
characterization equipment and the micromanipulators. All measurements are
carried out in air at room temperature.
5.2.1 Current-Voltage Measurement
The current-voltage characteristics of the devices, such as the output and transfer
characteristics of the transistors, is measured by using a semiconductor parameter
analyzer that is equipped with several source-measurement units (SMUs). Each
SMU can supply a constant current or a constant voltage and, at the same time,
measure the current and the voltage. For standard electrical characterisation, each
terminal of the device is connected to an SMU.
The output characteristics (see Fig. 4.3a) are measured as follows: The drain
current is measured as the drain voltage is swept, or actually changed in small
steps, from a starting value (0 V) to an end value, while the gate voltage is kept
constant. This is repeated for a number of, normally equally spaced, gate
The transfer characteristics (see Fig. 4.3b.) are measured in similar manner.
The drain current is measured while the gate voltage is swept and the drain
voltage is held constant. The gate voltage is swept over a range that extends from
the off-state to the on-state. This measurement is normally performed for a small
and a large drain voltage in order to record the drain current in the linear regime
and the saturation regime.
In both measurements, the sweeping parameter is often swept from the starting
value, to the end value, and then back again to the starting value (a dual sweep).
This is done in order to investigate if any hysteresis can be found in the I-V
5.2.2 Transient Measurements
The switching characteristics of the transistors were measured by using the setup
displayed in Figure 5.4a. In this measurement, the voltage drop V
over a resistor
inserted between the source contact and ground is recorded with an oscilloscope,
while the potential at the drain contact is held at a constant potential V
DC power supply and a square voltage pulse V
is applied to the gate electrode
with an arbitrary waveform generator. The source current I
The value of the resistance R is selected so that only a fraction of the applied
drain voltage is dropped over the resistor, i.e. |V
| ≪ |V
The recorded source current is the sum of two contributions: an exponentially
decaying current originating from the charging of the gate capacitor, i.e. the
charging current, and the current that flows between the source and the drain
contact, i.e. the transistor channel current. The charging current dominates the
recorded current immediately after that the gate voltage has been changed or
applied. Thus, the initial build-up (or disruption) of the transistor channel is not
measureable. However, if the drain contact is grounded, the recorded source
current will only consist of the charging current component, since the channel
current evidently is zero. Thus, the channel current can be extracted by taking the
difference between the source currents recorded for V
≠ 0 and V
= 0, as
illustrated in Figure 5.4b.
Figure 5.4 (a) Circuit schematic of the measurement setup used in the transient
measurements. (b) Illustration of how the channel current can be extracted from
the transient curves.
5.2.3 Impedance Spectroscopy
Impedance spectroscopy is a powerful technique to characterize the electrical
properties of various materials including those of electrolytes. The material to be
tested is sandwiched between two electrodes, thus forming a capacitor. The
impedance of the sample is measured by applying an alternating voltage with a
fixed frequency f to the capacitor. This will generate an alternating current of the
same frequency. There will generally be a phase shift between the current and
voltage signals, which can be described by the phase angle θ. The amplitude and
the phase shift of the current signal are measured for a number of frequencies in a
given range, usually going from high to low frequencies. This allows for
expressing the impedance as function of frequency. The frequency-dependent
complex impedance of the sample is given by
! 0) – I
where U* is the complex applied voltage and I* is the complex measured current.
The complex impedance can be expressed as a sum of a real and an imaginary
The phase angle can then be written as
In order to calculate the effective capacitance of the sample, an equivalent circuit
has to be chosen that reflects the behaviour of the sample. The equivalent circuit
either consists of a capacitor in series or in parallel with a resistor. The
capacitance for the first alternative is called the serial capacitance C
other is called the parallel capacitance C
, and they can be calculated according
6 Conclusions and Future Outlook
This thesis is entirely focused on organic thin-film transistors that employ
electrolytes as the gate insulator. The application of a gate bias will polarize the
electrolyte. Ions in the electrolyte will accumulate at the semiconductor interface
and form a so-called electric double layer (EDL) together with oppositely
charged electronic charge carriers in the organic semiconductor layer, which
have been injected from the source contact. The very small distance (in the order
of angstroms) between the two charged layers results in a very high capacitance,
typically in the order of tens of µF cm
, which allows the transistors to operate
at low voltage, around 1 V. Interestingly, the capacitance is virtually independent
on the thickness of the electrolyte layer. This is advantageous when it comes to
manufacturing of the transistors. It also means that the position of the gate
electrode becomes less critical, which opens up for alternative transistor designs.
For example, an electrolyte-gated transistor could be formed at the junction
between two microfibers (Paper V), or the transistor could be gated via a droplet
of pure water (Paper VI).
A question was raised in the introduction, whether it is possible to have a
confined EDL at the electrolyte-semiconductor interface or not. To address this
issue, we have used polyelectrolytes as the gate insulator material (Paper I–IV).
Polyelectrolytes are polymers that consist of charged polymer chains and mobile
counterions. Thus, polyelectrolytes dominantly transport ions of only one
polarity, and can therefore be referred to as either n- or p-type, analogous to n-
and p-doped semiconductors. In the reported transistors, the polyelectrolyte is
matched with the organic semiconductor such that the mobile ions are depleted
from the electrolyte-semiconductor interface when the transistor is operated in
the accumulation mode. In other words, p-type polyanions are used in p-channel
transistors and n-type polycations are used in n-channel transistors.
Consequently, during transistor operation, the EDL at this interface will be
composed of polyions in the gate insulator and electronic charges in the
semiconductor. The polyions are, due to their size, virtually immobile and cannot
penetrate into the semiconductor. Hence, these material combinations suppress
electrochemical doping of the semiconductor bulk, which implies that just
interfacial charging takes place. This statement is supported by that the observed
current levels are moderate, that very little hysteresis are observed in the current-
voltage characteristics and that the transistors display relatively fast switching
(≤ 100 µs).
A special feature of these transistors is that the switching speed saturates as
the channel length is reduced. This deviation from the downscaling rule is
explained by that the ionic relaxation in the electrolyte will limit the channel
formation rather than the electronic transport in the semiconductor. However, a
benefit with using an electrolyte as the gate insulator in transistors with small
channel lengths is that the high electric field in the EDL suppresses short-channel
effects (Paper II).
The use of solid electrolytes makes it possible to manufacture integrated
circuits. Unipolar circuits based on polyanion-gated p-channel transistors that
operated at voltages down to 0.9 V and display signal propagation delays down
0.3 ms per stage have been made (Paper III). The successful demonstration of
both p- and n-channel polyelectrolyte-gated transistors also allows for making
low-voltage complementary integrated circuits. Such demonstrated circuits
operate at supply voltages down to 0.2 V, have a static power consumption of
less than 2.5 nW per logic gate and display signal propagation delays down to
0.26 ms per stage (Paper IV).
The low operating voltage, relatively fast operating speed and low power
consumption make these polyelectrolyte-gated organic thin-film transistors a
promising candidate for use in printed electronics applications. However, there
are still a few hurdles to overcome before that can become reality. For example,
there are challenges with printing hydrophilic polyelectrolytes on strongly
hydrophobic semiconductor surfaces, or vice versa. This may require the use of
adhesion promoting layers or the use of specially synthesized polyelectrolyte and
organic semiconductor materials. Another challenge is to accomplish short
channel lengths with printed source and drain electrodes. Hence, in order to
obtain acceptable circuit speeds, high-mobility semiconductors have to be
employed. Moreover, the operating speed of the demonstrated transistors is
limited by the polarization of the polyelectrolytes. Increasing the ionic
conductivity of these layers should make these transistor circuits even faster.
 J. Bardeen, W. H. Brattain, Physical Review 1948, 74, 230.
 H. Shirakawa, E. J. Louis, A. G. MacDiarmid, C. K. Chiang, A. J. Heeger,
J. Chem. Soc., Chem. Commun. 1977, 578.
 A. J. Heeger, Chem. Soc. Rev. 2010, 39, 2354.
 A. C. Arias, J. D. MacKenzie, I. McCulloch, J. Rivnay, A. Salleo, Chem.
Rev. 2010, 110, 3.
 D. Tobjörk, R. Österbacka, Adv. Mater. 2011, 23, 1935.
 J. E. Anthony, A. Facchetti, M. Heeney, S. R. Marder, X. Zhan, Adv.
Mater. 2010, 22, 3876.
 J. H. Burroughes, D. D. C. Bradley, A. R. Brown, R. N. Marks, K.
Mackay, R. H. Friend, P. L. Burns, A. B. Holmes, Nature 1990, 347, 539.
 T. Ameri, G. Dennler, C. Lungenschmied, C. J. Brabec, Energy Environ.
Sci. 2009, 2, 347.
 C. N. Hoth, P. Schilinsky, S. A. Choulis, C. J. Brabec, Nano Letters 2008,
 D. A. Bernards, R. M. Owens, G. G. Malliaras, Organic Semiconductors
in Sensor Applications, Springer, New York 2008.
 H. Sirringhaus, Adv. Mater. 2005, 17, 2411.
 H. Klauk, Chem. Soc. Rev. 2010, 39, 2643.
 L. W. F. Chaves, C. Decker, "A survey on organic smart labels for the
Internet-of-Things", presented at 7th International Conference on
Networked Sensing Systems (INSS), 2010, Kassel, Germany, 2010.
 I. Ferreira, B. Br·s, J. I. c. Martins, N. Correia, P. Barquinha, E. Fortunato,
R. Martins, Electrochim. Acta 2011, 56, 1099.
 M. Hilder, B. Winther-Jensen, N. B. Clark, J. Power Sources 2009, 194,
 O. Bubnova, Z. U. Khan, A. Malti, S. Braun, M. Fahlman, M. Berggren,
X. Crispin, Nat Mater 2011, 10, 429.
 Y. Xuan, X. Liu, S. Desbief, Lecl, egrave, P. re, M. Fahlman, R.
Lazzaroni, M. Berggren, J. Cornil, D. Emin, X. Crispin, Phys. Rev. B
2010, 82, 115454.
 M. Bohm, A. Ullmann, D. Zipperer, A. Knobloch, W. H. Glauert, W. Fix,
"Printable electronics for polymer RFID applications", San Francisco, CA,
United states, 2006.
 D. Nilsson, M. Chen, T. Kugler, T. Remonen, M. Armgarth, M. Berggren,
Adv. Mater. 2002, 14, 51.
 D. Nilsson, N. Robinson, M. Berggren, R. Forchheimer, Adv. Mater. 2005,
 H. Klauk, U. Zschieschang, M. Halik, J. Appl. Phys. 2007, 102, 074514.
 H. Klauk, U. Zschieschang, J. Pflaum, M. Halik, Nature 2007, 445, 745.
 P. Bergveld, Sens. Actuators B 2003, 88, 1.
 G. Tzamalis, V. Lemaur, F. Karlsson, P. O. Holtz, M. Andersson, X.
Crispin, J. Cornil, M. Berggren, Chem. Phys. Lett. 2010, 489, 92.
 O. D. Jurchescu, J. Baas, T. T. M. Palstra, Appl. Phys. Lett. 2004, 84,
 W. Warta, N. Karl, Phys. Rev. B 1985, 32, 1172.
 H. Bässler, Phys. Status Solidi A 1993, 175, 15.
 M. C. J. M. Vissenberg, M. Matters, Phys. Rev. B: Condens. Matter
Mater. Phys. 1998, 57, 12964.
 G. Horowitz, R. Hajlaoui, P. Delannoy, J. Phys. III 1995, 5, 355.
 H. Yan, Z. Chen, Y. Zheng, C. Newman, J. R. Quinn, F. Dotz, M. Kastler,
A. Facchetti, Nature 2009, 457, 679.
 H. Sirringhaus, P. J. Brown, R. H. Friend, M. M. Nielsen, K. Bechgaard,
B. M. W. Langeveld-Voss, A. J. H. Spiering, R. A. J. Janssen, E. W.
Meijer, P. Herwig, D. M. de Leeuw, Nature 1999, 401, 685.
 H. Sirringhaus, N. Tessler, R. H. Friend, Science 1998, 280, 1741.
 M. S. A. Abdou, F. P. Orfino, Y. Son, S. Holdcroft, J. Am. Chem. Soc.
1997, 119, 4518.
 I. McCulloch, M. Heeney, M. L. Chabinyc, D. DeLongchamp, R. J. Kline,
M. Cölle, W. Duffy, D. Fischer, D. Gundlach, B. Hamadani, R. Hamilton,
L. Richter, A. Salleo, M. Shkunov, D. Sparrowe, S. Tierney, W. Zhang,
Adv. Mater. 2009, 21, 1091.
 I. McCulloch, M. Heeney, C. Bailey, K. Genevicius, I. MacDonald, M.
Shkunov, D. Sparrowe, S. Tierney, R. Wagner, W. Zhang, M. L.
Chabinyc, R. J. Kline, M. D. McGehee, M. F. Toney, Nature Mater. 2006,
 H. Ohkita, S. Cook, Y. Astuti, W. Duffy, S. Tierney, W. Zhang, M.
Heeney, I. McCulloch, J. Nelson, D. D. C. Bradley, J. R. Durrant, J. Am.
Chem. Soc. 2008, 130, 3030.
 H. S. Tan, N. Mathews, T. Cahyadi, F. R. Zhu, S. G. Mhaisalkar, Appl.
Phys. Lett. 2009, 94, 263303.
 Z. Bao, A. J. Lovinger, J. Brown, J. Am. Chem. Soc. 1998, 120, 207.
 R. Hagiwara, K. Matsumoto, Y. Nakamori, T. Tsuda, Y. Ito, H.
Matsumoto, K. Momota, J. Electrochem. Soc. 2003, 150, D195.
 Y. He, P. G. Boswell, P. Buhlmann, T. P. Lodge, J. Phys. Chem. B 2007,
 R. Marcilla, F. Alcaide, H. Sardon, J. A. Pomposo, C. Pozo-Gonzalo, D.
Mecerreyes, Electrochem. Commun. 2006, 8, 482.
 J. H. Cho, J. Lee, Y. He, B. Kim, T. P. Lodge, C. D. Frisbie, Adv. Mater.
2008, 20, 686.
 K. Tybrandt, K. C. Larsson, A. Richter-Dahlfors, M. Berggren, Proc. Natl.
Acad. Sci. U. S. A. 2010, 107, 9929.
 A. Kaltbeitzel, S. Schauff, H. Steininger, B. Bingol, G. Brunklaus, W. H.
Meyer, H. W. Spiess, Solid State Ionics 2007, 178, 469.
 O. Larsson, E. Said, M. Berggren, X. Crispin, Adv. Funct. Mater. 2009,
 A. M. Stephan, Eur. Polym. J. 2006, 42, 21.
 Y. J. Lee, B. Bingol, T. Murakhtina, D. Sebastiani, W. H. Meyer, G.
Wegner, H. W. Spiess, J. Phys. Chem. B 2007, 111, 9711.
 D. C. Grahame, Chem. Rev. 1947, 41, 441.
 L. Herlogsson, X. Crispin, N. D. Robinson, M. Sandberg, O.-J. Hagel, G.
Gustafsson, M. Berggren, Adv. Mater. 2007, 19, 97.
 H. Yuan, H. Shimotani, J. Ye, S. Yoon, H. Aliah, A. Tsukazaki, M.
Kawasaki, Y. Iwasa, J. Am. Chem. Soc. 2010, 132, 18402.
 J. E. Lilienfeld, United States Patent 1745175, Method and apparatus for
controlling electric currents, 1930.
 D. Kahng, United States Patent 3102230, Electric field controlled
semiconductor device, 1963.
 H. S. White, G. P. Kittlesen, M. S. Wrighton, J. Am. Chem. Soc. 1984,
 A. Tsumura, H. Koezuka, T. Ando, Appl. Phys. Lett. 1986, 49, 1210.
 G. Horowitz, Synth. Met. 2003, 138, 101.
 J. Zaumseil, H. Sirringhaus, Chem. Rev. 2007, 107, 1296.
 G. Horowitz, in Semiconducting Polymers, Vol. 2 (Eds: G. Hadziioannou,
G. C. Malliaras), Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim,
 E. J. Meijer, C. Tanase, P. W. M. Blom, V. E. Van, B. H. Huisman, L. D.
M. De, T. M. Klapwijk, Appl. Phys. Lett. 2002, 80, 3838.
 D. Boudinet, G. Le Blevennec, C. Serbutoviez, J.-M. Verilhac, H. Yan, G.
Horowitz, J. Appl. Phys. 2009, 105, 084510.
 Y.-Y. Noh, N. Zhao, M. Caironi, H. Sirringhaus, Nature Nanotech. 2007,
 F. Ante, F. Letzkus, J. Butschke, U. Zschieschang, K. Kern, J. N.
Burghartz, H. Klauk, "Submicron Low-Voltage Organic Transistors and
Circuits Enabled by High-Resolution Silicon Stencil Masks", presented at
International Electron Devices Meeting (IEDM), 2010, Piscataway, NJ,
 A. R. Brown, C. P. Jarrett, D. M. de Leeuw, M. Matters, Synth. Met. 1997,
 S. De Vusser, S. Steudel, K. Myny, J. Genoe, P. Heremans, "High-
performance low voltage organic thin-film transistors", Warrendale, PA
15086, United States, 2005.
 F. Eder, H. Klauk, M. Halik, U. Zschieschang, G. Schmid, C. Dehm, Appl.
Phys. Lett. 2004, 84, 2673.
 J. Ficker, A. Ullmann, W. Fix, H. Rost, W. Clemens, J. Appl. Phys. 2003,
 W. Fix, A. Ullmann, J. Ficker, W. Clemens, Appl. Phys. Lett. 2002, 81,
 S. H. Han, S. M. Cho, J. H. Kim, J. W. Choi, J. Jang, M. H. Oh, Appl.
Phys. Lett. 2006, 89, 093504.
 L. Herlogsson, M. Cölle, S. Tierney, X. Crispin, M. Berggren, Adv. Mater.
2010, 22, 72.
 T. D. Anthopoulos, D. M. De Leeuw, E. Cantatore, P. Van't Hof, J. Alma,
J. C. Hummelen, J. Appl. Phys. 2005, 98, 054503.
 T. D. Anthopoulos, B. Singh, N. Marjanovic, N. S. Sariciftci, A.
Montaigne Ramil, H. Sitter, M. Colle, D. M. De Leeuw, Appl. Phys. Lett.
2006, 89, 213504.
 F. Ante, U. Zschieschang, R. T. Weitz, D. Kalblein, K. Kern, H. Klauk,
"Low-voltage metal-gate top-contact organic thin-film transistors and
complementary inverters with submicron channel length", presented at
Device Research Conference - Conference Digest, DRC, 2009.
 K.-J. Baeg, D. Khim, D.-Y. Kim, S.-W. Jung, J. B. Koo, I.-K. You, H.
Yan, A. Facchetti, Y.-Y. Noh, J. Polym. Sci., Part B: Polym. Phys 2011,
 D. Bode, K. Myny, B. Verreet, B. van der Putten, P. Bakalov, S. Steudel,
S. Smout, P. Vicca, J. Genoe, P. Heremans, Appl. Phys. Lett. 2010, 96, 3.
 B. K. Crone, A. Dodabalapur, R. Sarpeshkar, R. W. Filas, Y. Y. Lin, Z.
Bao, J. H. O'Neill, W. Li, H. E. Katz, J. Appl. Phys. 2001, 89, 5125.
 M. Kitamura, Y. Kuzumoto, S. Aomori, Y. Arakawa, Appl. Phys. Express
 H. Klauk, M. Halik, U. Zschieschang, F. Eder, D. Rohde, G. Schmid, C.
Dehm, IEEE Trans. Electron Devices 2005, 52, 618.
 Y. Y. Lin, A. Dodabalapur, R. Sarpeshkar, Z. Bao, W. Li, K. Baldwin, V.
R. Raju, H. E. Katz, Appl. Phys. Lett. 1999, 74, 2714.
 J. H. Na, M. Kitamura, Y. Arakawa, Thin Solid Films 2009, 517, 2079.
 B. Yoo, T. Jung, D. Basu, A. Dodabalapur, B. A. Jones, A. Facchetti, M.
R. Wasielewski, T. J. Marks, Appl. Phys. Lett. 2006, 88, 082104.
 U. Zschieschang, F. Ante, M. Schlorholz, K. Kern, H. Klauk,
"Deterministic and continuous control of the threshold voltage and noise
margin of organic thin-film transistors and organic complementary circuits
using mixed phosphonic acid self-assembled monolayer gate dielectrics",
presented at Device Research Conference, 2009. DRC 2009, 22-24 June
 R. A. Street, A. Salleo, Appl. Phys. Lett. 2002, 81, 2887.
 D. J. Gundlach, L. Zhou, J. A. Nichols, T. N. Jackson, P. V. Necliudov, M.
S. Shur, J. Appl. Phys. 2006, 100, 024509.
 T. J. Richards, H. Sirringhaus, J. Appl. Phys. 2007, 102, 094510.
 L. Bürgi, T. J. Richards, R. H. Friend, H. Sirringhaus, J. Appl. Phys. 2003,
 C.-A. Di, G. Yu, Y. Liu, X. Xu, Y. Song, Y. Wang, Y. Sun, D. Zhu, H.
Liu, X. Liu, D. Wu, Appl. Phys. Lett. 2006, 88, 121907.
 J. Collet, O. Tharaud, A. Chapoton, D. Vuillaume, Appl. Phys. Lett. 2000,
 J. Z. Wang, Z. H. Zheng, H. Sirringhaus, Appl. Phys. Lett. 2006, 89,
 K. Tsukagoshi, F. Fujimori, T. Minari, T. Miyadera, T. Hamano, Y.
Aoyagi, Appl. Phys. Lett. 2007, 91, 113508.
 M. D. Austin, S. Y. Chou, Appl. Phys. Lett. 2002, 81, 4431.
 J. Liu, L. Herlogsson, A. Sawatdee, P. Favia, M. Sandberg, X. Crispin, I.
Engquist, M. Berggren, Appl. Phys. Lett. 2010, 97, 103303.
 S. Scheinert, T. Doll, A. Scherer, G. Paasch, I. Horselmann, Appl. Phys.
Lett. 2004, 84, 4427.
 N. Stutzmann, R. H. Friend, H. Sirringhaus, Science 2003, 299, 1881.
 M. Leufgen, A. Lebib, T. Muck, U. Bass, V. Wagner, T. Borzenko, G.
Schmidt, J. Geurts, L. W. Molenkamp, Appl. Phys. Lett. 2004, 84, 1582.
 C. W. Sele, T. Von Werne, R. H. Friend, H. Sirringhaus, Adv. Mater.
2005, 17, 997.
 N. Zhao, M. Chiesa, H. Sirringhaus, Y. Li, Y. Wu, B. Ong, J. Appl. Phys.
2007, 101, 064513.
 L. Herlogsson, Y.-Y. Noh, N. Zhao, X. Crispin, H. Sirringhaus, M.
Berggren, Adv. Mater. 2008, 20, 4708.
 J. N. Haddock, X. Zhang, S. Zheng, Q. Zhang, S. R. Marder, B. Kippelen,
Org. Electron. 2006, 7, 45.
 A. Facchetti, M. H. Yoon, T. J. Marks, Adv. Mater. 2005, 17, 1705.
 J. Veres, S. D. Ogier, S. W. Leeming, D. C. Cupertino, S. M. Khaffaf,
Adv. Funct. Mater. 2003, 13, 199.
 L.-L. Chua, J. Zaumseil, J.-F. Chang, E. C. W. Ou, P. K. H. Ho, H.
Sirringhaus, R. H. Friend, Nature 2005, 434, 194.
 M.-H. Yoon, H. Yan, A. Facchetti, T. J. Marks, J. Am. Chem. Soc. 2005,
 M. Zirkl, A. Haase, A. Fian, Sch, H. n, C. Sommer, G. Jakopic, G.
Leising, nther, B. Stadlober, I. Graz, N. Gaar, Schw, R. diauer, S. Bauer-
Gogonea, S. Bauer, Adv. Mater. 2007, 19, 2241.
 Y. Fujisaki, M. Mamada, D. Kumaki, S. Tokito, Y. Yamashita, Jpn. J.
Appl. Phys. 2009, 48, 111504 (5 pp.).
 L. A. Majewski, R. Schroeder, M. Grell, Adv. Funct. Mater. 2005, 15,
 M. Halik, H. Klauk, U. Zschieschang, G. Schmid, C. Dehm, M. Schutz, S.
Maisch, F. Effenberger, M. Brunnbauer, F. Stellacci, Nature 2004, 431,
 J. M. Ball, P. H. Wobkenberg, F. B. Kooistra, J. C. Hummelen, D. M. de
Leeuw, D. D. C. Bradley, T. D. Anthopoulos, Synth. Met. 2009, 159, 2368.
 S. Chao, M. S. Wrighton, J. Am. Chem. Soc. 1987, 109, 2197.
 S. Chao, M. S. Wrighton, J. Am. Chem. Soc. 1987, 109, 6627.
 M. Taniguchi, T. Kawai, Appl. Phys. Lett. 2004, 85, 3298.
 H. Shimotani, H. Asanuma, J. Takeya, Y. Iwasa, Appl. Phys. Lett. 2006,
 J. Takeya, K. Yamada, K. Hara, K. Shigeto, K. Tsukagoshi, S. Ikehata, Y.
Aoyagi, Appl. Phys. Lett. 2006, 88, 112102.
 M. J. Panzer, C. D. Frisbie, J. Am. Chem. Soc. 2005, 127, 6960.
 M. J. Panzer, C. R. Newman, C. D. Frisbie, Appl. Phys. Lett. 2005, 86,
 M. J. Panzer, C. D. Frisbie, Adv. Funct. Mater. 2006, 16, 1051.
 M. J. Panzer, C. D. Frisbie, Appl. Phys. Lett. 2006, 88, 203504.
 M. J. Panzer, C. D. Frisbie, J. Am. Chem. Soc. 2007, 129, 6599.
 A. S. Dhoot, J. D. Yuen, M. Heeney, I. McCulloch, D. Moses, A. J.
Heeger, Proc. Natl. Acad. Sci. U. S. A. 2006, 103, 11834.
 J. D. Yuen, A. S. Dhoot, E. B. Namdas, N. E. Coates, M. Heeney, I.
McCulloch, D. Moses, A. J. Heeger, J. Am. Chem. Soc. 2007, 129, 14367.
 E. Said, X. Crispin, L. Herlogsson, S. Elhag, N. D. Robinson, M.
Berggren, Appl. Phys. Lett. 2006, 89, 143507.
 S. Ono, S. Seki, R. Hirahara, Y. Tominari, J. Takeya, Appl. Phys. Lett.
2008, 92, 103313.
 S. Ono, K. Miwa, S. Seki, J. Takeya, Appl. Phys. Lett. 2009, 94, 063301.
 T. Uemura, M. Yamagishi, S. Ono, J. Takeya, Appl. Phys. Lett. 2009, 95,
103301 (3 pp.).
 T. Uemura, M. Yamagishi, S. Ono, J. Takeya, Japanese Journal of
Applied Physics 2010, 49, 01AB13 (3 pp.).
 T. Fujimoto, M. M. Matsushita, K. Awaga, Chem. Phys. Lett. 2009, 483,
 J. Lee, M. J. Panzer, Y. He, T. P. Lodge, C. D. Frisbie, J. Am. Chem. Soc.
2007, 129, 4532.
 J. H. Cho, J. Lee, Y. Xia, B. Kim, Y. He, M. J. Renn, T. P. Lodge, C. D.
Frisbie, Nature Mater. 2008, 7, 900.
 J. Lee, L. G. Kaake, J. H. Cho, X.-Y. Zhu, T. P. Lodge, C. D. Frisbie, J.
Phys. Chem. C 2009, 113, 8972.
 Y. Xia, J. Cho, B. Paulsen, C. D. Frisbie, M. J. Renn, Appl. Phys. Lett.
2009, 94, 013304.
 D. Braga, M. Ha, W. Xie, C. D. Frisbie, Appl. Phys. Lett. 2010, 97,
 Y. Xia, W. Zhang, M. Ha, J. H. Cho, M. J. Renn, C. H. Kim, C. D. Frisbie,
Adv. Funct. Mater. 2010, 20, 587.
 M. Hamedi, L. Herlogsson, X. Crispin, R. Morcilla, M. Berggren, O.
Inganos, Adv. Mater. 2009, 21, 573.
 S. W. Lee, H. J. Lee, J. H. Choi, W. G. Koh, J. M. Myoung, J. H. Hur, J. J.
Park, J. H. Cho, U. Jeong, Nano Lett. 2010, 10, 247.
 L. Kergoat, L. Herlogsson, D. Braga, B. Piro, M.-C. Pham, X. Crispin, M.
Berggren, G. Horowitz, Adv. Mater. 2010, 22, 2565.
 L. Seung-Yong, C. Gyoung-Rin, L. Hyuneui, L. Kyung-Mi, L. Sang-
Kwon, Appl. Phys. Lett. 2009, 95, 013113 (3 pp.).
 H. Shimotani, G. Diguet, Y. Iwasa, Appl. Phys. Lett. 2005, 86, 22104.
 K. H. Lee, S. Zhang, T. P. Lodge, C. D. Frisbie, J. Phys. Chem. B 2011,
 P. Andersson, R. Forchheimer, P. Tehrani, M. Berggren, Adv. Funct.
Mater. 2007, 17, 3074.
 P. Andersson, D. Nilsson, P. O. Svensson, M. Chen, A. Malmström, T.
Remonen, T. Kugler, M. Berggren, Adv. Mater. 2002, 14, 1460.
 L. G. Kaake, Y. Zou, M. J. Panzer, C. D. Frisbie, X. Y. Zhu, J. Am. Chem.
Soc. 2007, 129, 7824.
 T. Mills, L. G. Kaake, X. Y. Zhu, Appl. Phys. A: Mater. Sci. Process.
2009, 95, 291.
Low operating voltages for p-channel organic
field-effect transistors (OFETs) can be achieved
by using an electrolyte as the gate insulator.
However, mobile anions in the electrolyte can lead
to undesired electrochemistry in the channel. In
order to avoid this, a polyanionic electrolyte is
used as the gate insulator. The resulting OFET
has operating voltages of less than 1 V (see
figure) and shows fast switching (less than 0.3 ms)
in ambient atmosphere.
A polyelectrolyte is used as gate insulator
material in organic field-effect transistors with
self-aligned inkjet printed sub–micrometer
channels. The small separation of the charges in
the electric double layer at the electrolyte-
semiconductor interface, which builds up in tens of
microseconds, provides a very high transverse
electric field in the channel that effectively
suppresses short-channel effects at low applied
A polyanionic electrolyte is used as gate
insulator in top-gate p-channel polymer thin-film
transistors. The high capacitance of the
polyelectrolyte film allows the transistors and
integrated circuits to operate below 1.5 V. Seven-
stage ring oscillators that operate at supply
voltages down to 0.9 V and exhibit signal
propagation delays as low as 300 µs per stage are
Organic complementary inverters and ring
oscillators based on polyelectrolyte-gated thin-
film transistors are demonstrated. Detrimental
electrochemical doping is suppressed by using
polyanionic and polycationic gate insulators in the
p- and n-channel transistors, respectively. The
circuits operate at supply voltages between 0.2 V
and 1.5 V, have a static power consumption of
less than 2.5 nW per logic gate and show
propagation delays down to 0.26 ms per stage.
Electrolyte-gate organic field-effect transistors
embedded at the junction of textile microfibers are
demonstrated. The fiber transistor operates below
1 V, and delivers large current densities. The
transience of the organic thin-film transistor's
current and the impedance spectroscopy
measurements reveal that the channel is formed
in two steps.
High-dielectric-constant insulators, organic
monolayers, and electrolytes have been
successfully used to generate organic field-effect
transistors operating at low voltages. Here, we
report on a device gated with pure water. By
replacing the gate dielectric by a simple water
droplet, we produce a transistor that entirely
operates in the field-effect mode of operation at
voltages lower than 1 V. This result creates
opportunities for sensor applications using water-
gated devices as transducing medium.